Fatigue Testing. Objectives


 Winfred McKinney
 1 years ago
 Views:
Transcription
1 Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students are required to construct an SN curve (stress level  number of cycles to failure) of the test samples provided. Students can define the fatigue endurance limit or fatigue life and fatigue strength of the materials. Students are able to interpret the obtained experimental results and use them as a tool for material selection in engineering applications. Mechanical Metallurgy Laboratory
2 1. Literature Review 1.1 Characteristics of fatigue failure Most engineering failures are mainly due to fatigue in which the components are subjected to fluctuating or cyclic loading such as suspended bridges, rails, or airplane wings. Though the fluctuating load is normally less than the yield strength of the materials, it results in fracture behaviour which is more severe than that achieved from static loading. Fatigue failures are therefore unpredictable, and provide highrisk situations, if the operators are not aware of material behaviour when subjected to fatigue loading. Fatigue failures can be easily observed from its unique characteristics of fracture surfaces, revealing as a beach mark pattern as shown in figure 1 (a). Fatigue failures are also driven by severe environment. For example, corrosion fatigue is a combined situation of fatigue loading in a corrosive environment as illustrated in figure 1 (b). 1.2 Stress cycles and the SN curve Figure 1: Fatigue surfaces. Cyclic loading in general has no repeated patterns or in situations where overloading occurs as seen in figure 2 (a). However, in order to investigate the fatigue behaviour according to engineering purposes, a simple relation between stress and number of cycles to failure (time) can be expressed in a sinusoidal curve as illustrated in figure 2 (b). Fatigue behaviour of materials can thus be practically described according to the parameters given as follows; Mechanical Metallurgy Laboratory
3  Maximum stress (σ max )  Minimum stress (σ min )  Stress range ( σ) = σ max σ min  Mean stress = (σ max + σ min )/2  Stress amplitude = (σ max σ min )/2  Stress ratio = σ min /σ max Figure 2: Relationships between stress and time or no. of cycles. These parameters significantly affect the fatigue behaviours of the materials. This is for example, increasing in the maximum stress as well as mean stress and stress range leads to more severe fatigue conditions. If the maximum and minimum stresses are tensile, they are considered to be more dangerous than compressive stresses as the tensile stresses will open up the fatigue crack. Furthermore, if the maximum and minimum stresses are in similar amounts but having the opposite signs (tensile and compressive stresses), the stresses in this case is called completely reversed cyclic stresses in which the stress ratio equals 1. For instance, a rotatingbeam fatigue machine as shown in figure 3, fitted with a fatigue specimen hung by a weight in the middle. Specimen rotating action is driven by a motor on the right results in tensile stress in the lower fibrous and compressive stress in the upper fibrous of the specimen gauge length. Therefore, along the gauge length, specimen will be subjected to alternating tensile and compressive stresses similar to the reversed cyclic loading. The specimen will be fatigue loaded until failure. The number of cycles to failure according to the cyclic stress applied will then be recorded. Mechanical Metallurgy Laboratory
4 Figure 3: Rotatingbeam fatigue testing machine [2]. The fatigue testing can also be conducted using an instrument as shown in figure 4. The fatigue specimen is gripped on to a motor at one end to provide the rotational motion whereas the other end is attached to a bearing and also subjected to a load or stress. When the specimen is rotated about the longitudinal axis, the upper and the lower parts of the specimen gauge length are subjected to tensile and compressive stresses respectively. Therefore, stress varies sinusoially at any point on the specimen surface. The test proceeds until specimen failure takes place. The revolution counter is used to obtain the number of cycles to failures corresponding to the stress applied. Figure 4: Fatigue testing machine [3]. Increasing of the weight applied to the fatigue specimen results in a reduction in number of cycles to failure. We can then use the experimental results to construct an SN curve as illustrated in figure 5. The fatigue test is normally conducted using at least 812 specimens in order to provide sufficient information for the interpretation of fatigue behaviour of the tested material. The SN curve shows a relationship between the applied stress and the number of cycles to failure, which can be used to determine the fatigue life of the material subjected to cyclic loading. High applied cyclic stress results in a low number of cycles to failure. For example, the fatigue testing of a 1047 steel provides a small number of cycles to failure at a high cyclic stress. As the cyclic stress reduces, the number of Mechanical Metallurgy Laboratory
5 cycles to failure increases. At the fatigue endurance limit, there will be a certain value of the cyclic stress where specimen failure will not occur. This cyclic stress level is called the fatigue strength. According to figure 4, the fatigue strength of 1047 steel is approximately 320 MPa. However, nonferrous alloys such as some alloys of aluminium, magnesium and copper will not normally show the fatigue endurance limit. The slope can be found gradually downwards with increasing number of cycles to failure and shows no horizontal line. In such a case, the fatigue strength will be defined at a stress level where the number of cycles to failure reaches 10 7 or 10 8 cycles. The fatigue strength of engineering materials is in general lower than their tensile strength. A ratio of the fatigue strength to the tensile strength as described in equation 1 is called the fatigue ratio. It is normally observed that, in the case of steels, the fatigue strength increases in proportional to the tensile stress. Therefore, improving the tensile strength by hardening or other heat treatments normally increases the fatigue strength of the mateiral. However for nonferrous metals such as aluminium alloys, the fatigue ratio is found approximately 0.3 and the improvement of the tensile strength do not necessary increases the fatigue strength of the material. Fatigue strength Fatigue ratio = (1) Tensile strength Figure 5: SN curves of 1047 steel and 2014T6 aluminium alloy[2]. Mechanical Metallurgy Laboratory
6 The fatigue SN curve are generally considered in 2 cases, which are high cycle fatigue and low cycle fatigue. The study of high cycle fatigue concerns about fatigue behaviour of the materials which is controlled by the applied load or stress and where the gross deformation taking place is elastic. However highly localized plastic deformation can also be observed for example at the crack tip. The number of cycles to failure in this case is normally determined at higher than 10 5 cycles. The SN curve in the high cycle fatigue region can be expressed using the Basquin equation as follow; N σ p = C (2) a where σ a is Stress amplitude p and C is Empirical constants In the case of low cycle fatigue, the fatigue behaviour is controlled by elastic and plastic strains and the number of cycles leading to failure is lower than 10 4 or 10 5 cycles. Gross plastic deformation is due to high levels of the applied stresses and leads to difficulties for stress interpretation. The low cycle fatigue data is generally presented as a relationship between plastic strain ( ε p ) and the number of cycles to failure (N) as illustrated in figure 6. When plotted in a loglog scale, the relationship can be expressed following the CoffinManson relationship ε 2 p = ε (2N) ' f c (3) where ε p /2 is Plastic strain amplitude ε f is Fatigue ductility coefficient 2N is Strain reversal to failure, whereby 1 cycle equals 2 reversals C is Fatigue ductility exponent, having the values ranging from 0.5 to 0.7. Mechanical Metallurgy Laboratory
7 Figure 6: Low cycle fatigue curve ( ε p vs N) 347 stainless steel [1]. 1.3 Cyclic stressstrain curve Materials response differently to static and cyclic loading as illustrated from stressstrain relationship. If we first consider figure 7 (a), which shows the stressstrain loop under controlled strain (at constant strain amplitude), the stressstrain relation follows the OAB line when subjected to tensile loading passing the yield point. On unloading, the stressstrain relation follows BC line and goes into the compressive region having a negative strain. It is noticed that the compressive yield is somewhat smaller than that obtained from the tensile yielding. This phenomenon is called the Baushinger effect. Reloading results in a hysteresis loop and gives a total strain ε = ε e + ε p where ε e is the elastic strain range and ε p is the plastic strain range as shown in figure 7 (a). Furthermore, plastic deformation taking place during cyclic loading causes microstructural changes such as structure and density of dislocations. Therefore, after every cycle applied, the material responses slightly differently to the cyclic loading. The material will experience either cyclic hardening or cyclic softening, and both change the shape of the hysteresis loop as illustrated in figure 8. The hysteresis loop generally stabilizes after being cyclic loaded about 100 cycles. Figure 7 (b) demonstrates how materials response differently to static loading and cyclic loading. The former shows a momotonic σ ε curve whereas the latter provides a cyclic σ ε curve. This cyclic σ ε curve is constructed by connecting the tip of the stablized hysteresis loops obtained from a number of fatigue tests at different controlled strain amplitude. Moreover, the cyclic σ ε curve can also be expressed in a power curve analogy to that obtained from static loading as shown in equation 4. Mechanical Metallurgy Laboratory
8 ' ' n σ = ( ) (4) K ε p where n K is the cyclic strain hardening exponent is the cyclic strength coefficient Figure 7: a) Stressstrain loop for constant strain cycling and b) comparison of momotonic and cyclic stressstrain curve for a cyclic hardening materials[1]. Figure 8: Responses of metals to cyclic strain cycles[1]. Mechanical Metallurgy Laboratory
9 1.4 Characteristics of fatigue surfaces Fatigue surfaces normally show no gross plastic deformation and exhibit relatively flat fracture surfaces as shown previously in figure 1 (a). The so called beach mark pattern is often well recognized on the fatigue surfaces on the macroscopic scale. However, if we examine the fatigue fracture surface using a high magnification scanning electron microscope (SEM), we can notice a number of minute striations as depicted in figure 9. These striations are normally observed in the stable fatigue crack growth region. Some metals might not show evident traces of these striations. Figure 9: Fatigue surface examined using a scanning electron microscope, showing the fatigue striations. The striations in the stable fatigue crack propagation are found to be related to the fatigue cycles applied. The occurrence of these striations is due to the plastic blunting process as illustrated in figure 10. If we consider the cross section of the fatigue crack, we will find that the crack is closed at the initial stage or when the minimum stress is applied. During the load increment, the fatigue crack will open according to the amount of the load applied. During crack opening, slips occur in the vicinity of both ends of the crack tips as seen from the arrows. This results in plastic deformation around the fatigue crack tip. When the load reaches the maximum values, plastic blunting process takes place, yielding the maximum crack opening distance as seen at stage 3 from figure 10. After unloading, crack closing takes place and the reversed slips now occur at the crack tips. Finally, the fatigue crack goes back to the initial stage of crack closer but with an increment of one striation as noticed from fatigue crack in stages 1 and 5 respectively. Mechanical Metallurgy Laboratory
10 Figure 10: Plastic blunting model for fatigue striation [4 ]. 1.5 Factors influencing fatigue properties of materials As mentioned previously, characteristics of the applied stresses such as maximum stress, mean stress and stress ratio significantly affects the fatigue behavior of the materials. However, there are a range of factors which are also found to significantly influence the fatigue properties of engineering materials. These are for example, stress concentration, size effect, surface effect, combined stresses, cumulative fatigue and sequence effect, metallurgical variables, corrosion and temperature. Generally, the fatigue crack initiations are observed near the surface. Rough surfaces are therefore undesirable due to stress concentration which accounts for further fatigue crack propagation and eventually lead to global failure. Corrosive environment and high service temperatures are reckoned to have negative effects on fatigue properties of the materials as they accelerate faster rates of both fatigue initiation and propagation. Mechanical Metallurgy Laboratory
11 Figure 11: Fatigue testing machine in the laboratory [4]. Figure 12: Fatigue specimen [4]. Mechanical Metallurgy Laboratory
12 2. Materials and equipment 2.1 Fatigue specimens 2.2 Micrometer or vernier caliper 2.3 Permanent pen 2.4 Fatigue testing machine 3. Experimental Procedure 3.1 Measure dimensions of brass and steel specimens provided and record in tables 1 and 2. If the distance from the load end to the minimum diameter of the specimen is mm, the bending stress, σ, can be calculated the bending stress for a load P (N) is shown in equation P 32 = 3 π D σ (5) 3.2 Conduct the fatigue test at room temperature using the fatigue testing machine as shown in figure 11. Fit one end of the specimen to a motor and fit the other end to a bearing hung with a known weight, indicating the stress applied to the specimen. Start the motor to rotate the specimen at a constant speed. The revolution counter is used to record the number of cycles to which the specimen fails. Record the result in table 1 and Change the weights used and follow the experiment in 2.2. Again, record the results in tables 1 and Construct the SN curves of the steel specimens. 3.5 Investigate fracture surfaces of broken fatigue specimen and sketch the result in tables 1 and Analyze, discuss the obtained results. Give conclusions. Mechanical Metallurgy Laboratory
13 4. Results Details Specimen 1 Specimen 2 Specimen 3 Specimen 4 Specimen 5 Specimen diameter (mm) Crosssectional areas (mm 2 ) Weight (kg) Maximum stress (MPa) Frequeny (Hz) No. of cycles to failure (cycles) Fracture surfaces Table 1: Fatigue data of steel specimens. Mechanical Metallurgy Laboratory
14 Figure 13: SN curve of steel specimens. Mechanical Metallurgy Laboratory
15 5. Discussion Mechanical Metallurgy Laboratory
16 6. Conclusions Mechanical Metallurgy Laboratory
17 7. Questions 7.1 Explain the fatigue endurance limit. What is the obtained fatigue strength in steels? 7.2 Predict the fatigue strength of aluminium. Give reasons. Mechanical Metallurgy Laboratory
18 7.3 Explain the differences between fatigue failure and cleavage fracture. 8. References 8.1 Dieter, G.E., Mechanical metallurgy, 1988, SI metric edition, McGrawHill, ISBN Hashemi, S. Foundations of materials science and engineering, 2006, 4 th edition, McGraw Hill, ISBN ก, ก Engineering materials, 2549, ก ( ), ISBN10: Roberts, N.P., HiTech instruction manual, HSM19 mk3: Rotating fatigue machine, Mechanical Metallurgy Laboratory
Tensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationdifferent levels, also called repeated, alternating, or fluctuating stresses.
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationFigure 1: Typical SN Curves
StressLife Diagram (SN Diagram) The basis of the StressLife method is the Wohler SN diagram, shown schematically for two materials in Figure 1. The SN diagram plots nominal stress amplitude S versus
More informationHardness Testing. Objectives
Laboratory 2 Hardness Testing Objectives Students are required to understand the principles of hardness testing, i.e., Rockwell, Brinell and Vickers hardness tests. Students are able to explain variations
More informationPLASTIC DEFORMATION AND STRESSSTRAIN CURVES
PLASTIC DEFORMATION AND STRESSSTRAIN CURVES Introduction Background Unit: Plastic Deformation and StressStrain Curves In the last unit we studied the elastic response of materials to externally applied
More informationFatigue. 3. Final fracture (rough zone) 1. Fatigue origin. 2. Beach marks (velvety zone)
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
More information9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationTensile Testing of Steel
C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0  INTRODUCTION See General Lab Report Format
More informationFatigue Failure Due to Variable Loading
Fatigue Failure Due to Variable Loading Daniel Hendrickson Department of Computer Science, Physics, and Engineering University of Michigan Flint Advisor: Olanrewaju Aluko 1. Abstract Fatigue failure in
More informationMechanical Metallurgy
Mechanical Metallurgy Lecturer Assessment Dr. Assignment 20 (homework, quiz, attendance) Midterm exam 40 Final exam 40 Total 100 Mechanical Metallurgy Subject of interests Part I Mechanical fundamentals
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationFATIGUE CONSIDERATION IN DESIGN
FATIGUE CONSIDERATION IN DESIGN OBJECTIVES AND SCOPE In this module we will be discussing on design aspects related to fatigue failure, an important mode of failure in engineering components. Fatigue failure
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationPrinciples of Fracture Mechanics
81 CHAPTER 8 FAILURE PROBLEM SOLUTIONS Principles of Fracture Mechanics 8.1 This problem asks that we compute the magnitude of the maximum stress that exists at the tip of an internal crack. Equation
More informationPlastic Behaviour  Tensile Strength
Plastic Behaviour  Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hotrolled, coldrolled, heat treated, etc.).
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More informationExperiment: Fatigue Testing
Experiment: Fatigue Testing Objectives  To demonstrate the use of the Instron servohydraulic testing machine for testing specimens subjected to cyclic (fatigue) loadings.  To analytically approximate
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationSAMPLE FORMAL LABORATORY REPORT. Fatigue Failure through Bending Experiment Adapted from a report submitted by Sarah Thomas
SAMPLE FORMAL LABORATORY REPORT Fatigue Failure through Bending Experiment Adapted from a report submitted by Sarah Thomas Lab Partners: David Henry and James Johnson ME 498 November 10, 2004 Professor
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationσ y ( ε f, σ f ) ( ε f
Typical stressstrain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A =  A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationTensile Testing Laboratory
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationHow Management Decisions Make or Break Plant Uptime
How Management Decisions Make or Break Plant Uptime Abstract How Management Decisions Make of Break Plant Uptime: When you run machines above design rates that decision goes against all that we know about
More informationFATIGUE TESTS AND STRESSLIFE (SN) APPROACH
FATIGUE TESTS AND STRESSLIFE (SN) APPROACH FATIGUE TESTING LOADING TEST MACHINES SPECIMENS STANDARDS STRESSLIFE APPEROACH SN CURVES MEAN STRESS EFFECTS ON SN BEHAVIOR FACTORS INFLUENCING SN BEHAVIOR
More informationFatigue of Metals Copper Alloys. Samuli Heikkinen 26.6.2003
Fatigue of Metals Copper Alloys Samuli Heikkinen 26.6.2003 T 70 C Temperature Profile of HDS Structure Stress amplitude 220 MPa Stress Profile of HDS Structure CLIC Number of Cycles f = 100 Hz 24 hours
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationProperties of Materials
CHAPTER 1 Properties of Materials INTRODUCTION Materials are the driving force behind the technological revolutions and are the key ingredients for manufacturing. Materials are everywhere around us, and
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationMIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE
MIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE Introduction In this experiment, the finite life fatigue behavior of a smooth cylindrical specimen as shown in Figure 1 will be studied in
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationPROPERTIES OF MATERIALS
1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties
More informationB.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN
No. of Printed Pages : 7 BAS01.0 B.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) CV CA CV C:) O TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN Time : 3 hours Maximum Marks : 70 Note : (1)
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationInteraction of Hydrogen and Deformation in 316L Stainless Steel
Proceedings of the SEM Annual Conference June 14, 2009 Albuquerque New Mexico USA 2009 Society for Experimental Mechanics Inc. Interaction of Hydrogen and Deformation in 316L Stainless Steel Bonnie R.
More informationLecture 14. Chapter 81
Lecture 14 Fatigue & Creep in Engineering Materials (Chapter 8) Chapter 81 Fatigue Fatigue = failure under applied cyclic stress. specimen compression on top bearing bearing motor counter flex coupling
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationFATIGUE FROM VARIABLE AMPLITUDE LOADING. Ali Fatemi  University of Toledo All Rights Reserved Chapter 9 Variable Amplitude Loading 1
FATIGUE FROM VARIABLE AMPLITUDE LOADING Ali Fatemi  University of Toledo All Rights Reserved Chapter 9 Variable Amplitude Loading 1 FATIGUE FROM VARIABLE AMPLITUDE LOADING SPECTRUM LOADS AND CUMULATIVE
More informationDESIGN TO PREVENT FATIGUE
W H I T E P A P E R DESIGN TO PREVENT FATIGUE Overview In 1954, two crashes involving the world s first commercial airliner, the de Havilland Comet, brought the words metal fatigue to newspaper headlines
More informationLong term performance of polymers
1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form
More informationExperiment F: Failure Analysis
Experiment F: Failure Analysis Introduction: In this experiment, a component that has failed in service will be analyzed to determine the probable cause or causes of the failure. Each group will give a
More informationG1RTCT200105071 D. EXAMPLES F. GUTIÉRREZSOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION
D. EXAMPLES 316 WORKED EXAMPLE I Infinite Plate under fatigue Introduction and Objectives Data Analysis 317 INTRODUCTION AND OBJECTIVES One structural component of big dimensions is subjected to variable
More informationThe Truth About Actuator Life: Screw Drive Survival
The Truth About Actuator Life: Screw Drive Survival By Tolomatic, Inc. About the Author: Tolomatic is a leading supplier of linear actuators, both electric and pneumatically driven. Tolomatic's expertise
More informationPhysics 3 Summer 1989 Lab 7  Elasticity
Physics 3 Summer 1989 Lab 7  Elasticity Theory All materials deform to some extent when subjected to a stress (a force per unit area). Elastic materials have internal forces which restore the size and
More information1.Adapted from Gordon, J.E., Structures or why things don t fall down, Da Capo Press, Inc., New York, N.Y., 1978, Chapter 15.
Lecture 4: Cyclic loading and fatigue Safe working life: 1 All structures will be broken or destroyed in the end just as all people will die in the end. It is the purpose of medicine and engineering to
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationCompletely reversed, strain controlled fatigue tests of a steel alloy with E=210000 MPa resulted in the following data:
Kul49.4350 Fatigue o Structure Example solutions 5 Problem 51. Completely reversed, strain controlled atigue tests o a steel alloy with E=10000 resulted in the ollowing data: a a, (o the stable curve)
More informationFatigue crack propagation
1 (20) Repetition Ð Crack initiation and growth Small cracks Shear driven Interact with microstructure Mostly analyzed by continuum mechanics approaches Large cracks Tension driven Fairly insensitive to
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationINFLUENCE OF SHOT PEENING ON CHROMIUM ELECTROPLATED AISI 4340 STEEL FATIGUE STRENGTH
INFLUENCE OF SHOT PEENING ON CHROMIUM ELECTROPLATED AISI 4340 STEEL FATIGUE STRENGTH *Voorwald, H. J. C., Silva, M. P., Costa, M. Y. P., a Pigatin, L. W., Marques, B. M. F. Fatigue and Aeronautic Research
More informationMechanics of MaterialsSteel
Mechanics of MaterialsSteel Structural Steel Structural steel considered one of the predominant materials for construction of buildings, bridges, towers and other structures. The preferable physical properties
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationME311 Machine Design
ME Machine Design Lecture 5: FullyReversing Fatigue and the SN Diagram W Dornfeld Oct26 Fairfield University School of Engineering Discovering Fatigue With the Industrial Revolution came the steam engine
More informationPOWER SCREWS (ACME THREAD) DESIGN
POWER SCREWS (ACME THREAD) DESIGN There are at least three types of power screw threads: the square thread, the Acme thread, and the buttress thread. Of these, the square and buttress threads are the most
More informationANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON ENERGY DISSIPATION
EPJ Web of Conferences 6, 6 38009 (00) DOI:0.05/epjconf/000638009 Owned by the authors, published by EDP Sciences, 00 ANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationMUKAVEMET KIRILMA HİPOTEZLERİ
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More informationRolling  Introductory concepts
Rolling  Introductory concepts R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 8 Table of Contents 1. Rolling 
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationAnalysis of Fatigue Fracture Surfaces in Aluminum Alloy 2024 T351
International Journal of Mining, Metallurgy & Mechanical Engineering (IJMMME) Volume, Issue (03) ISSN 30 400 (Online) Analysis of Fatigue Fracture Surfaces in Aluminum Alloy 04 T35 Benguediab Mohamed,
More informationVolume 54 2009 Issue 2 MLCF AN OPTIMISED PROGRAM OF LOWCYCLE FATIGUE TEST TO DETERMINE MECHANICAL PROPERTIES OF CAST MATERIALS
A R C H I V E S O F M E T A L L U R G Y A N D M A T E R I A L S Volume 54 2009 Issue 2 M. MAJ,J.PIEKŁO MLCF AN OPTIMISED PROGRAM OF LOWCYCLE FATIGUE TEST TO DETERMINE MECHANICAL PROPERTIES OF CAST MATERIALS
More informationLecture 18 Strain Hardening And Recrystallization
138 Lecture 18 Strain Hardening And Recrystallization Strain Hardening We have previously seen that the flow stress (the stress necessary to produce a certain plastic strain rate) increases with increasing
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationRESILIENT MODULUS: WHAT, WHY, AND HOW?
RESILIENT MODULUS: WHAT, WHY, AND HOW? Shane Buchanan, Vulcan Materials Company, 08/1/07 Resilient modulus (M r ) continues to be a key design parameter for pavement systems. Accurate knowledge of the
More informationDevelopment of Ushaped Steel Damper for Seismic Isolation System
UDC 624. 042. 7 Development of Ushaped Steel Damper for Seismic Isolation System Kazuaki SUZUKI* 1 Atsushi WATANABE* 1 Eiichiro SAEKI* 1 Abstract Seismic isolation system was widely admitted after HanshinAwaji
More informationExamination of failed landing gear struts MD Helicopters, Model MD520N VHMPI 21 June 2004
Appendix A: Technical Analysis Report Examination of failed landing gear struts MD Helicopters, Model MD520N VHMPI 21 June 2004 Report No. 35/04 Task No. BE/200400015 Occurrence No. BO/200402243 Page
More informationCitation Journal of Constructional Steel Research, 2014, v. 96, p
Title The Art of Coupon Tests Author(s) Huang, Y; Young, B Citation Journal of Constructional Steel Research, 014, v. 96, p. 159175 Issued Date 014 URL http://hdl.handle.net/107/00516 Rights NOTICE: this
More informationFatigue Life Estimates Using Goodman Diagrams
Fatigue Life Estimates Using Goodman Diagrams by Robert Stone The purpose of this paper is to review the proper methods by which spring manufacturers should estimate the fatigue life of a helical compression
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationEFFECT OF SEVERE PLASTIC DEFORMATION ON STRUCTURE AND PROPERTIES OF AUSTENITIC AISI 316 GRADE STEEL
EFFECT OF SEVERE PLASTIC DEFORMATION ON STRUCTURE AND PROPERTIES OF AUSTENITIC AISI 316 GRADE STEEL Ladislav KANDER a, Miroslav GREGER b a MATERIÁLOVÝ A METALURGICKÝ VÝZKUM, s.r.o., Ostrava, Czech Republic,
More informationUltrasonic Technique and Device for Residual Stress Measurement
Ultrasonic Technique and Device for Residual Stress Measurement Y. Kudryavtsev, J. Kleiman Integrity Testing Laboratory Inc. 80 Esna Park Drive, Units 79, Markham, Ontario, L3R 2R7 Canada ykudryavtsev@itlinc.com
More informationMechanical properties 3 Bend test and hardness test of materials
MME131: Lecture 15 Mechanical properties 3 Bend test and hardness test of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Bend test of brittle materials Hardness testing
More informationCHAPTER 4 TENSILE TESTING
CHAPTER 4 TENSILE TESTING EXERCISE 28, Page 7 1. What is a tensile test? Make a sketch of a typical load/extension graph for a mild steel specimen to the point of fracture and mark on the sketch the following:
More informationDescription of mechanical properties
ArcelorMittal Europe Flat Products Description of mechanical properties Introduction Mechanical properties are governed by the basic concepts of elasticity, plasticity and toughness. Elasticity is the
More informationFATIGUE LIFE OF BOLT SUBJECTED TO FATIGUE LOADING CONDITIONS
20 FATIGUE LIFE OF BOLT SUBJECTED TO FATIGUE LOADING CONDITIONS ABSTRACT K. Din and M. T. H. Ghazali Faculty of Civil Engineering, Universiti Teknologi MARA, Shah Alam, Malaysia Email: kdfila@hotmail.com
More informationEffect of Temperature and Aging Time on 2024 Aluminum Behavior
Proceedings of the XIth International Congress and Exposition June 25, 2008 Orlando, Florida USA 2008 Society for Experimental Mechanics Inc. Effect of Temperature and Aging Time on 2024 Aluminum Behavior
More informationMaterial Deformations. Academic Resource Center
Material Deformations Academic Resource Center Agenda Origin of deformations Deformations & dislocations Dislocation motion Slip systems Stresses involved with deformation Deformation by twinning Origin
More informationHardness Test. Subjects of interest
Hardness Test Chapter 9 Subjects of interest Introduction/objectives Brinell hardness Meyer hardness Vickers hardness Rockwell hardness Microhardness tests Relationship between hardness and the flow curve
More informationDamage due to fatigue occurs when loading is markedly varying in time. R decreases with time S T. MSÚ F max
5. Fatigue of steel structures Fatigue loading, Wöhler s approach and fracture mechanics, fatigue strength, influence of notches, damage accumulation, Eurocode approach. Damage due to fatigue occurs when
More informationUniversity of Portland School of Engineering LABORATORY OUTLINE: TENSILE TESTING OF STEEL & ALUMINUM ALLOYS (ASTM E8)
TENSILE TESTING OF STEEL & ALUMINUM ALLOYS (ASTM E8) To carry out a standard tensile test on specimens of a hot rolled steel (AISI 1045), Type 2024 T351 aluminum, polymers (UHMWPE, acrylic) and, from
More information